living radical polymerization by polyhedral oligomeric silsesquioxane-holding initiators: ...
Post on 02-Feb-2017
Embed Size (px)
Living Radical Polymerization by Polyhedral OligomericSilsesquioxane-Holding Initiators: Precision Synthesis ofTadpole-Shaped Organic/Inorganic Hybrid Polymers
Kohji Ohno, Satoshi Sugiyama, Kyoungmoo Koh, Yoshinobu Tsujii,Takeshi Fukuda,*, Mikio Yamahiro, Hisao Oikawa, Yasuhiro Yamamoto,Nobumasa Ootake, and Kenichi Watanabe
Institute for Chemical Research, Kyoto University, Uji, Kyoto 611-0011, Japan, and Goi ResearchCenter, Chisso Petrochemical Corporation, 5-1 Goi-Kaigan, Ichihara, Chiba 290-8551, Japan
Received June 8, 2004; Revised Manuscript Received September 8, 2004
ABSTRACT: Incompletely condensed polyhedral oligomeric silsesquioxane (POSS) with the highly reactivegroup of trisodium silanolate was used for the synthesis of two initiators for atom transfer radicalpolymerization, one with a 2-bromoisobutyl group and the other with a chlorosulfonyl group. Theseinitiators were applied to solution polymerizations of styrene and methyl methacrylate in the presenceof a copper complex. In both systems, polymerization proceeded in a living fashion, as indicated by thefirst-order kinetics of monomer consumption, the evolution of molecular weight in direct proportion tomonomer conversion, the good agreement of molecular weight with the theoretical one, and the lowpolydispersity, thus providing tadpole-shaped polymers with an inorganic head of POSS and an organictail of well-defined polymer. Thermogravimetric and differential scanning calorimetric studies showedthat both thermal degradation and glass transition temperatures of the organic/inorganic hybrid polymerswith molecular weights up to about 20 000 were enhanced as compared to those of model polymers withoutthe POSS moiety.
Polyhedral oligomeric silsesquioxanes (POSSs), cube-octameric molecules with Si-O-Si framework, haveattracted much interest as a nanoscale building blockfor the construction of organic/inorganic hybrid materi-als.1 Strategies have been made for the synthesis ofhybrid materials by incorporating POSSs into polymersto improve their thermal and mechanical properties asa result of homogeneously dispersing inorganic sub-stances into polymers at the nanometer level.2,3 Vinylmonomers with a pendant group of POSSs were copo-lymerized with a variety of monomers.4 POSSs func-tionalized with reactive groups such as epoxy, amine,isocyanate, and vinyl ones were used as a cross-linkerto produce cross-linked hybrid polymers.5,6 Poly(ethyl-ene oxide) (PEG)-functionalized POSS was synthesizedby the reaction of octahydrido-POSS with allyl-PEG inthe presence of a Pt catalyst.7 Hybrid polyoxazolineswere synthesized by ring-opening polymerization of2-methyl-2-oxazoline with an initiator-functionalizedPOSS.8 Atom transfer radical polymerization (ATRP)9,10was also applied to the synthesis of POSS-based hybridpolymers.11,12 Matyjaszewski et al. showed that a com-mercially available benzyl chloride-holding POSS servedas an initiator for ATRP of styrene (S), yielding poly-styrenes (PSs) having a POSS moiety at the end ofpolymer chain.12 Laine et al. reported that a starpolymer having a POSS core was synthesized by ATRPof methyl methacrylate (MMA) initiated by an octafunc-tional POSS initiator.13
Incompletely condensed POSS, which has a trisilanolmoiety at one corner of the cubelike framework, is a
fascinating compound because it undergoes corner-capping reaction with chlorosilanes, transition metalcomplexes, and metal alkyl complexes so as to producea wide variety of functional POSSs.14,15 Very recently,we developed an efficient method for the synthesis ofincompletely condensed POSS with the highly reactivegroup of trisodium silanolate, heptaphenyltricyclohep-tasiloxane trisodium silanolate (7Ph-T7-(ONa)3, Scheme1). The reaction of 7Ph-T7-(ONa)3 with varied types oftrichlorosilanes proceeded much faster and more selec-tively than the conventional one using the trisilanolgroup, thus giving the desired products in a high yield.16
The goal of this study is to demonstrate that 7Ph-T7-(ONa)3 can be used to produce a more efficient andversatile initiator for copper-mediated ATRP for thesynthesis of well-defined, tadpole-shaped polymerichybrids with a POSS at the end of polymer chain. Thiswill be illustrated by the synthesis of two types ofinitiators that will eventually yield POSS-carrying low-polydispersity polymers with a wide range of molecularweights. The thermal properties of the resultant hybridswill also be demonstrated in terms of glass transitionand thermal degradation temperatures.
Experimental SectionMaterials. Ethyl 2-bromoisobutylate (98%, 2-(EiB)Br) was
used as received from Nacalai Tesque Inc., Osaka, Japan.L-Sparteine (99%, Sp) was purchased from Aldrich and usedwithout further purification. Methyl methacrylate (99%, MMA)and styrene (99%, S) were obtained from Nacalai Tesque Inc.and purified by distillation under reduced pressure overcalcium hydride. 2-(4-Chlorosulfonylphenyl)ethyltrichlorosilane(50% in dichloromethane, CTS) was obtained from Gelest Inc.7Ph-T7-(ONa)3 was prepared as described in the patent.16 Allother reagents were purchased from commercial sources andused as received.
Measurements. Gel permeation chromatographic (GPC)analysis was carried out at 40 C on a high-speed liquid
Institute for Chemical Research, Kyoto University. Goi Research Center, Chisso Petrochemical Corp.* To whom correspondence should be addressed. E-mail:
8517Macromolecules 2004, 37, 8517-8522
10.1021/ma048877w CCC: $27.50 2004 American Chemical SocietyPublished on Web 10/21/2004
chromatography system (Shodex GPC-101) equipped with aguard column (Shodex GPC KF-G), two 30 cm mixed columns(Shodex GPC KF-804L, exclusion limit ) 400 000), and adifferential refractometer (Shodex RI-101). Tetrahydrofuran(THF) was used as an eluent at a flow rate of 0.8 mL/min.Poly(methyl methacrylate) (PMMA) and polystyrene (PS)standards were used to calibrate the GPC system. Nuclearmagnetic resonance (1H, 13C, and 29Si NMR) spectra wereobtained on a JEOL/AL400 400 MHz spectrometer. Thermo-gravimetric analysis (TGA) was performed on a Perkin-ElmerTGA 7 thermogravimetric analyzer. Measurements were car-ried out under a continuous flow of He gas from 50 to 800 Cat the heating rate 20 C/min. The degradation temperatureTdeg was defined as the point of the maximum mass decrementrate. Differential scanning calorimetry (DSC) was performedon a Perkin-Elmer DSC 7 under a N2 atmosphere. Theinstrument was calibrated with known standards: indium (Tm) 156.6 C) and zinc (Tm ) 419.5 C). The sample was heatedfrom 50 to 180 C at the rate 200 C/min and kept at 180 Cfor 5 min and then cooled to 10 C at the rate -200 C/min.After the sample was kept at 10 C for 3 min, measurementwas carried out with the scan rate of 10 C/min within thetemperature range 10-150 C. The glass transition temper-ature Tg was obtained at the midpoint of the specific heatincrement.
Synthesis of 2-(4-Chlorosulfonylphenyl)ethylhepta-phenyl-T8-silsesquioxane (7Ph-T8-CSPE, Scheme 1). 50wt % of CTS in dichloromethane (10.17 g, 15 mmol of CTS)was quickly added to a cold solution of 7Ph-T7-(ONa)3 (10 g,10 mmol) in dry THF (200 mL) at 0 C. The mixture wasmagnetically stirred for 1 h at 0 C. The resultant precipitatewas removed by filtration, and the filtrate was concentratedby a rotary evaporator to obtain a slightly yellow oil. Theresidue was diluted with ethyl acetate (100 mL), and themixture was again concentrated by a rotary evaporator untila slightly cloudy solution was obtained. The system was cooledin a refrigerator to obtain a white solid, which was recrystal-lized from ethyl acetate (4.88 g, 42%). IR (KBr, cm-1): 1430and 1135-1090 (Si-Ph), 1380 and 1190 (-SO2Cl), and 1090-
1020 (Si-O-Si). 1H NMR (CDCl3, 400 MHz): 1.23 (t, 2H,Si-CH2-), 2.91 (t, 2H, -CH2-C6H4), 7.30-7.79 (m, 39 H, Si-C6H5 and -C6H4-SO2Cl). 13C NMR (CDCl3, 100 MHz): 13.0(Si-CH2-), 29.0 (-CH2-C6H4), 128.1, 130.2, 131.1, and 134.3(Si-C6H5), 127.2, 129.3, 142.0, 152.3 (-C6H4-SO2Cl). 29SiNMR (CDCl3, 79 MHz): -66.69 (-CH2-SiO1.5), -78.35,-78.41, and -78.67 (C6H5-SiO1.5). Anal. Calcd for C50H43O14-SClSi8: C, 51.77; H, 3.74. Found: C, 52.08; H, 3.74.
Synthesis of 2-Bromoisobutyryloxyethylheptaphenyl-T8-silsesquioxane (7Ph-T8-BIE, Scheme 1). 7Ph-T8-BIEwas synthesized via the three step reactions described below.First, 7Ph-T7-(ONa)3 (10 g, 10 mmol), triethylamine (1.5 g, 14.8mmol), and dry THF (200 mL) were charged into a round-bottom flask, to which acetoxyethyltrichlorosilane (3.3 g, 14.8mmol) was quickly added at room temperature. The mixturewas magnetically stirred for 2 h at room temperature and thenpoured into n-hexane (1 L) to obtain a crude product. Theresultant solid was redissolved in toluene (100 mL) andwashed three times with water (3 330 mL). The organic layerwas collected and dried over anhydrous MgSO4. After filtra-tion, ethanol (100 mL) was added into the filtrate to yieldacetoxyethylheptaphenyl-T8-silsesquioxane (7Ph-T8-AE) as awhite solid (6.88 g, 66%). IR (KBr, cm-1): 1740 (CdO), 1430and 1135-1090 (Si-Ph), 1240 (C-O), 1090-1000 (Si-O-Si).1H NMR (CDCl3, 400 MHz): 1.33-1.37 (t, 2H, Si-CH2-),1.84 (s, 3H, CH3-CdO), 4.28-4.32 (t, 2H, -O-CH2-), 7.31-7.46 and 7.72-7.82 (m, 35 H, Si-C6H5). 13C NMR (CDCl3, 100MHz): 13.2 (Si-CH2-), 20.8 (CH3-CdO), 60.6 (-O-CH2-), 128.1, 130.2, 131.0-130.1, and 134.3-130.4 (Si-C6H5), 171.2(CdO). 29Si NMR (CDCl3, 79 MHz): -67.97 (-CH2-SiO1.5),-78.36 and -78.67 (C6H5-SiO1.5).
Second step: 7Ph-T8-AE (2.58 g, 2.47 mmol), methanol (175mL), and chloroform (175 mL) were charged in a round-bottomed flask, to which concentrated H2SO4 (0.7 mL) wasadded at room temperature. The mixture was magneticallystirred for 72 h at room temperature and concentrated by arotary evaporator. The oily residue was redissolved in ethylacetate (500 mL) and washed twice with water